Injectable polypeptide hydrogel/inorganic nanoparticle composites for bone tissue engineering
Injectable polypeptide hydrogel/inorganic nanoparticle composites for bone tissue engineering
Wei-Shun HuangID 0 1
I-Ming ChuID 0 1
0 Editor: Bing Xu, Brandeis University , UNITED STATES
1 Department of Chemical Engineering, National Tsing Hua University , Hsinchu , Taiwan
The general concept of tissue engineering is to restore biological function by replacing defective tissues with implantable, biocompatible, and easily handleable cell-laden scaffolds. In this study, osteoinductive and osteoconductive super paramagnetic Fe3O4 nanoparticles (MNP) and hydroxyapatite (HAP) nanoparticles were incorporated into a di-block copolymer based thermo-responsive hydrogel, methoxy(polyethylene glycol)-polyalanine (mPA), at various concentrations to afford composite, injectable hydrogels. Incorporating nanoparticles into the thermo-responsive hydrogel increased the complex viscosity and decreased the gelation temperature of the starting hydrogel. Functionally, the integration of inorganic nanoparticles modulated bio-markers of bone differentiation and enhanced bone mineralization. Moreover, this study adopted the emerging method of using either a supplementary static magnetic field (SMF) or a moving magnetic field to elicit biological response. These results demonstrate that combining external (magnet) and internal (scaffold) magnetisms is a promising approach for bone regeneration.
Data Availability Statement: All relevant data are
within the manuscript file.
Funding: This work was supported by the grant
104-2221-E-007-126-MY3 from the Ministry of
Science and Technology (Taiwan). The funders had
no role in study design, data collection and
analysis, decision to publish, or preparation of the
Competing interests: The authors have declared
that no competing interests exist.
Trauma, bone disease, and tumor excision are common causes of critical-sized bone defects.
Currently, few synthetic bone grafts offer osteoconduction and osteoinduction properties
comparable to those of bone autographs, which have limited availability [
]. Therefore, bone
tissue engineering is a field of significant research interest. The general approach of bone tissue
engineering is to offer a biomimetic environment that supports cell adhesion, growth, and
proliferation; as well as provide proper physical (e.g., static magnetic field), chemical, and
biological (e.g., osteogenic genes, proteins, or cells) factors to support tissue regeneration [
Hydrogel is a soft matter with high water content which mimics the extracellular matrix
(ECM) found in the body [
]. Specific hydrogels are injectable and can be used to easily fill in
defects of various sizes and shapes while retaining their unique physical and biological
]. Peptide hybrid polymers are a promising new class of biomaterials developed to
combine the advantages of synthetic and peptide polymers, namely the ability of peptide
polymers to self-assemble into hierarchical structures and the simplicity and reproducibility in the
preparation of synthetic polymers [
]. However, in addition to high water content and
permeability for nutrients and oxygen, hydrogels used for bone tissue engineering must also
exhibit supportive properties for cell growth and differentiation. Composites that consist of
nanomaterials incorporated into a hydrogel are attractive for bone tissue engineering because
this strategy allows fine control of the mechanical, biological, and chemical properties of the
Among the nanomaterials, HAP and MNP are commonly employed in bone tissue
engineering because these materials have been shown to improve bone tissue mineralization when
incorporated into various scaffold materials [
]. In addition, they have been adopted specifically as
bioactive factors in hydrogels to improve mineralization and osteogenic differentiation [
Furthermore, MNP have been incorporated into different matrices to fabricate magnetic
]. In fact, many research groups have reported that weak magnetic or pulse
electromagnetic fields induce and promote bone fracture healing, spinal fusion, and bone ingrowth into
ceramics in animal models. Moreover, a strong static magnetic field of 0.1?10 T has been shown
to regulate the orientation of matrix proteins and cells in vitro and in vivo [
In this study, we introduced both HAP and MNP into a mPEG-poly(alanine) hydrogel to
provide bone tissue engineering scaffolds of suitable mechanical property and compatibility.
Then, magnetic stimulation was applied to explore the potential positive effects of this strategy
in combination with the composite approach. The performance was evaluated based on gene
expression and cell staining.
Materials and methods
Methoxy polyethylene glycol of Mw 2000 (mPEG), L-alanine, dimethyl sulfoxide (DMSO),
potassium hexacyanoferrate(II) trihydrate, trypsin-EDTA solution 0.25%, dexamethasone,
?glycerophosphate, ascorbic acid, iron (II) sulfate heptahydrate, iron (III) chloride, calcium
chloride, disodium hydrogen phosphate, phosphate buffer saline (PBS),
tetramethylammonium hydroxide (TMAH) solution (25 wt%), LIVE/DEAD assay kit and deuterated
trifluoracetic acid (TFA-d) were obtained from Sigma (St. Louis, MO). N,N-dimethylformamide
(DMF, Sigma- Aldrich), tetrahydrofuran (THF, Sigma-Aldrich), and chloroform
(Mallinckrodt) were dried over CaH2 before use. SYBR Green Real-time PCR Master Mix was received
from Applied Biosystems (Carlbad, CA). Primers were designed in lab and synthesized by
MDBio (Taipei, Taiwan). Alpha-minimum essential medium (?-MEM), fetal bovine serum
(FBS), antimycotics-antibiotics, gentamycin, and fungizone were purchased from Gibco.
Synthesis of di-block copolymer mPA
Methoxy polyethylene glycol-poly (alanine) (mPA) was synthesized by ring-opening
polymerization included amine-terminated mPEG and N-carboxyanhydride form of L-alanine. Protocols
used to prepare mPEG-NH2 and alanine-NCA (Ala-NCA) are similar to those described in a
previous study [
]. Briefly, 2.00 g (1mmol) of mPEG was dissolved in anhydrous chloroform/
DMF (100 mL; 2/1 v/v) and 4.86g (42.25 mmol) of Ala-NCA was added to the reaction mixture.
Polymerization was carried out at 25?C for 72 h under anhydrous nitrogen condition. The
theoretical molecule weight of synthesized mPA is 2000?3000. Finally, the product was precipitated,
dissolved in DMSO for dialysis against deionized water (MW cut of 3500), and lyophilized.
Synthesis of magnetic nanoparticles (MNP)
Fe3O4 MNP were synthesized by chemical co-precipitation, according to a described method,
with minor modification [
]. In the typical experimental procedure, MNP were fabricated by
2 / 17
mixing 10 mL of 1M ferric chloride hexahydrate (FeCl3?6H2O) with 5 mL of 1M ferrous
sulfate heptahydrate (FeSO4?7H2O) in a two- neck flask under nitrogen atmosphere. The solution
was stirred, followed by the dropwise addition of 20 ml of 25% (w/w) TMAH, until a pH of 13
was reached. Vigorous stirring was continued for 20 min. The solution color changed from
orange to black, as black precipitates formed. A permanent magnet was used to isolate the
black precipitated product and the supernatant was discarded. Deionized water was added for
washing to remove excess ions and tetramethyl ammonium salt in the suspension. This
washing procedure was repeated for three times. Finally, the washed precipitated product was
dispersed in deionized water and stored until further use.
Synthesis of hydroxyapatite nanoparticles
Hydroxyapatite (HAP) nanoparticles were synthesized using a method described previously
]. Briefly, 0.03M Na2HPO4 was added dropwise into 0.05M CaCl2 at 50?C and pH 10 with
a stirring speed of 300 rpm. After continuous stirring at 300 rpm for 24 h, the precipitated
product was harvested by centrifugation, washed, and dried. The final product was dispersed
in deionized water and stored until further investigation.
Preparation of MNP/mPA and HAP/mPA nanocomposite hydrogels
First, mPA was dissolved in deionized water at 4?C for 24 h to yield a 3 wt% solution. Next,
MNP and HAP suspensions were dispersed by a ultrasonicator (DC400, Delta, Taiwan) and
separately added into hydrogel solutions at different nanoparticle concentrations (0, 500, and
1000 ?g/mL). Then, the mixtures were added dropwisely into cell culture plates and cultured
for 10 min in a 37?C oven to afford nanocomposite hydrogels. Nanocomposite hydrogels
containing 500 ?g/mL of HAP and 1000 ?g/mL of MNP are denoted as H5/mPA and M10/mPA,
Copolymer mPA was dissolved in TFA-d prior to analysis. The composition and number
average molecular weight (Mn) were verified using a 500 MHz NMR spectrometer (Varian, USA).
Solution-gel (sol-gel) phase transition
The storage modulus of mPA, M10/mPA and H5/mPA in aqueous solutions (3.0 wt%) was
investigated by a rheometer (MCR 302, Anton Paar GmbH, Austria) at 4?C and 37?C. Briefly,
aqueous polymer solution was pipetted between parallel plates 25 mm in diameter with a gap
of 0.5 mm. During dynamic mechanical analysis, the sample was kept inside a chamber with
water-soaked cotton to minimize water evaporation. Data were collected under controlled
stress (30?) and frequency of 3.0 rads-1.
Fourier-transform infrared (FTIR) spectroscopy
The FTIR spectra of hydrogel solutions (3.0 wt% of mPA, M10/mPA, and H5/mPA in
deionized water) were obtained using a FTS-800 system (Thermo Fisher, USA) equipped with
attenuated total reflectance (ATR). The samples were balanced for 20 min at 37?C and spectra was
Transmission electron microscopy (TEM)
The nanoscale morphology of MNP and HAP was examined by TEM. For TEM analysis, an
instrument (H7100, Hitachi, Japan) operating at 120 keV was used. For sample preparation, a
3 / 17
drop of a diluted dispersion of MNP or HAP was placed on a Formvar coated copper grid and
left to dry on a filter paper. Before sample analysis, the copper grid was put into the drying
oven to ensure low moisture.
Scanning electron microscopy (SEM)
The pore structure and surface morphology of scaffolds were observed by SEM. Micrograph
images of gels at 37?C were taken after polymer aqueous solutions (1 mL, 3.0wt %) were
transferred from 25?C to 37?C and stored for 20 min in the oven. The gels were then quenched with
liquid nitrogen at ?196?C and freeze-dried. SEM images were obtained by a field emission
scanning electron microscopy instrument (JSM-6700F, JEOL Ltd., Japan).
Laser ablation inductively coupled mass spectrometry (LA-ICPMS)
The dispersion characteristic of inorganic nanoparticles in hydrogels was analyzed by
LA-ICPMS. Briefly, 100 ?L of the gel solution was transferred to a cover glass. The size and
shape of the test samples were similar to those formed using a 48 well plate. Then, the slide was
placed into the incubator to allow for gelation. A laser ablation system (Model: UP-213, New
Wave Re- search Inc., Fremont, CA, Nd:YAG 213 nm wavelength) was used for sample
ablation and the ablated fouling samples were introduced into a inductively coupled plasma mass
spectrometer (7500a ICP-MS, Agilent Technology, Inc. USA) for element determination. The
line scan mode was conducted under the following condition: a pulse rate of 10 Hz, a 150 ?m
diameter beam at a traveling velocity 100 ?m/s, energy output 4 J/cm2, focused spot size
110 ?m, transport Ar gas flow 1.01 L/min, dwell time 8 s, and intersite pause 1 s. The
LAICP-MS scan range was 3000 ?m ? 2850 ?m and a total of 900 lines covered the entire area of
the tested gel sample. The raw data obtained from LA-ICP-MS were converted into a
twodimensional (2D) image by using the MATrix LABoratory (MATLAB) software.
MC3T3-E1 pre-osteoblasts were cultured ?-MEM supplemented with 10% FBS and 1%
antibiotic/antimycotic. MC3T3-E1 pre-osteoblasts within passage 10 were used in this study to
ensure pre-osteoblastic characteristics. Cells were grown in a humidified atmosphere of 5%
CO2 at 37?C. The osteogenic media consisted of ?-MEM supplemented with 10 mM ?-glycerol
phosphate, 1 10?7 M dexamethasone, and 50 ?g/mL L-ascorbic acid. The culture medium was
changed every 3 day till the cell density reached 80?90% confluences. The supernatant was
then removed and cells washed with 10 mL of PBS three times to remove residuals from the
medium, followed by treatment with 0.25% trypsin-EDTA solution. A cell pellet was collected
after centrifugation at 750 rpm for 10 min, with supernatant discarded. A cell suspension was
made by mixing the cell pellet with 1 mL cell culture medium and re-suspended in three 100
mm tissue culture plates.
Gels encapsulated cells and in vitro culture
For the in-vitro hydrogels encapsulated-cells studies, mPA polymer was UV sterilized over
night. mPA polymer was dissolved in deionized water and mixed with different inorganic
nanoparticles as described above. After 3 days of culture, the cells were passaged and directly
encapsulated to the mPA, H5/mPA, and M10/mPA polymer solutions at a final concentration
of 5 103 cells/well. The solutions were manually mixed, and allowed to gel at 37?C in an
incubator for 30 min before in vitro culture. The cell-containing hydrogels and controls were
placed in 0.5 mL medium in 48-well tissue culture plates and cultured for 7, 14, and 21 days.
4 / 17
Medium was changed every 3 days by removing 250 ?L medium and replenishing 250 ?L fresh
medium. At the desired time points, samples were processed for Live/Dead staining and real
time RT-PCR assay (n = 3).
Cell viability in the HAP or MNP co-culture system with or without gel encapsulation was
determined using the LIVE/DEAD kit, respectively. At the desired time points, samples
from each system were followed by removal of the medium and PBS washing for three
times. The assay reagent was prepared by mixing 2 ?L ethidium homodimer-1 (4 10-6M)
and 1 ?L calcein acetoxy methyl ester (2 10?6 M) in 1mL PBS. Added 200 ?l reagent to
each well in 48-well plates for staining live (green) and dead (red) cells. The whole process
was performed in dark and incubated with the reagent at 37?C for 30 min. After the
incubation period, the stained cells were viewed under a fluorescent microscope. The
excitation/emission wavelength were 528/617 nm for ethidium homodimer-1 and 494/517 nm
for calcein acetoxy methyl ester.
Static magnetic field (SMF) exposure system
SMF-exposed cells and control cells were first placed in an incubator (NUAIRE, USA).
Neodymium (Nd2Fe14B) magnets with a diameter of 8 cm and a thickness of 1 cm were used to
produce the SMF. The average magnetic strength density on the surface was monitored by a
handheld Gauss meter (EFA 3; B-field sensor, Wandel & Goltermann, Germany) and was
shown to have an average strength of 0.4 T (range: 0.38?0.43 T). The density of SMF strength
is in the range suitable for clinical test. For all exposure experiments, cultured plates were
placed directly on the surface of the permanent magnets. Control cells were placed in the same
incubator, but in an area with magnetic strength similar to the natural environment. To probe
the effect of a moving magnetic field, we established a homemade moving magnetic system.
The same magnets were used as for the SMF test, but the cell culture plates were placed on an
orbital shaker inside the incubator. The daily magnetic exposure time and plate shake rate
were 1 hour and 100 rpm, respectively [
Cell proliferation and differentiation assay
For quantitative real-time polymerase chain reaction (PCR), the cell and cell-hydrogel were
added TRIsure reagent according to protocol to extract total RNA at predetermined time
points. Then, an all-in-one cDNA synthesis supermix kit was used for reverse transcription of
total RNA to cDNA, which was stored at -20?C prior to use. Three different genes were
analyzed including alkaline phosphatase (ALP), osteocalcin (OCN), and osteopontin (OPN) using
a real-time PCR system (ABI Prism 7300, Thermo Fisher, USA). Glyceraldehyde-3-phosphate
dehydrogenase (GAPDH) was selected as the housekeeping gene. Table 1 lists the primer
At least three replicates were performed for each test condition. The results were presented
with error bars as the mean +/- SD. Statistical analysis was performed using the Student?s
ttest, p values < 0.05 were considered as statistically significant.
5 / 17
Oliginucleotides sequence (5?- 3?)
Results and discussions
Synthesis of di-block copolymer mPA and characterization
The 1H-NMR spectrum of mPA is shown in Fig 1A. Five characteristic peaks in the spectrum
were used to calculate the molecular weight (Mn) and composition of the polymer. In the
NMR spectra, the methyl protons (CH-CH3) and methine protons (CO-CH-CH3-NH2) of
poly(alanine) at 1.4 to 1.6 ppm and 4.5 to 4.7 ppm, respectively, were correctly found to be at a
ratio of 3:1. The terminal methyl group at 1.6 to 1.7 ppm has a slightly downfield shift due to
its close proximity with amine. Methylene protons (O-CH2-CH2) and the terminal methyl
protons (CH3-O) of mPEG were found at 3.8 to 4.0 ppm and 3.5 ppm, respectively.
Mn and Mw of the copolymer were determined by GPC and 1H-NMR respectively. Using
the integration ratio between methylene protons on mPEG and methyl protons on
poly(alanine) Mw can be calculated, which was approximately 4500 Da.
The GPC of the mPA showed homogenous composition of the molecular weights with a
polydispersity index (Mw/Mn) of 1.09, and the number average molecular weight (Mn) and
weight-average molecular weight (Mw) determined with PEG standards are 2275 and 2490,
Finally, we selected 3.0 wt % injectable hydrogel solution in current study. The photographs
of the sol (4?C) and gel (37?C) states prepared from the injectable hydrogel solution (3.0 wt %)
are shown in Fig 1B.
Characterization of inorganic nanoparticles
TEM micrographs of HAP and MNP nanoparticles are shown in Fig 2. As revealed, the
microstructure of HAP nanoparticles was needle-like with a mean crystallite size of 10 nm in
diameter and 100?150 nm in length. The morphology of MNP nanoparticles was spherical with a
mean particle diameter of approximately 10 nm.
The stability of nanoparticles in suspension is controlled by hydrophobicity- hydrophilicity,
and van der Waals forces. Most biomedical applications require chemically stable and
uniformly sized nanoparticles that are well dispersed in water. In general, nanometer size particles
aggregate in suspension due to van der Waals forces in order to reduce the total surface or
interfacial energy. Consequently, such aggregation can hamper the efficacy of nanoparticles in
many applications such as drug delivery, catalysis, and detection due to low surface area and
large sizes [
]. Surface modification of nanoparticles can be carried out either during their
synthesis or in a post-synthesis process. Typically, polymers on the particle surface ensure
particle stability and improve its dispersibility [
]. These polymer coatings are generally
required to be biocompatible and hydrophilic. In this study, dispersive MNP was prepared by
reacting iron (II) and iron (III) in an ammonia solution with the addition of TMAH to
6 / 17
Fig 1. (A)1H-NMR spectrum of mPA (CF3COOD). (B) Photographs of sol (4?C) and gel (37?C) states of the injectable
Fig 2. TEM images of (A) MNP and (B) HAP; the diameter MNP was approximately 10 nm and the size of HAP was
approximately 10 nm in width and 100?150 nm in length.
7 / 17
Fig 3. Elemental mapping of inorganic nanoparticles in the hydrogel. (A and D: mPA, B: H5/mPA, C: H10/mPA, E:
M5/mPA, F: M10/mPA) Color bar on the right side indicates element intensity, with blue and red corresponding to
low and high concentration respectively.
chemically stabilize the MNP in a colloidal solution. For comparison, HAP was synthesized
without the addition of TMAH.
The dispersion of inorganic nanoparticles in the hydrogel
LA-ICP-MS is a powerful and direct solid-sampling analytical technique that allows for highly
sensitive and precise elemental and isotopic analysis of materials [
]. In this study,
LA-ICP-MS was adopted to observe the elemental distribution of encapsulated inorganic
nanoparticles in the hydrogels. Fig 3 shows the spatial distribution of studied elements in
mPA, M10/mPA and H5/mPA hydrogels. As observed, elemental distribution became
inhomogeneous when nanoparticle concentration was increased beyond 500 ?g/mL. On the other
hand, MNP were better distributed than HA at high concentration. In the H5/mPA group, the
intensity at most areas was 100 to 200. However, specific areas had an intensity difference of
approximately 2 to 5 times, indicating aggregation in local areas. In a comparison, the intensity
of M5/mPA was homogenous at a low concentration. The intensity difference of M10/mPA
was approximately 1.5 times, which is lower than those of of H5/mPA and H10/mPA. These
data suggest that HAP tends to aggregate in the hydrogel due to its hydrophobicity.
Cell toxicity of inorganic nanoparticles
Cell proliferation was studied after 7 days of co-culture with different concentrations of
inorganic nanoparticles. Fig 4 shows the LIVE/DEAD staining of MC3T3-E1 co-cultured with
different concentrations of HAP and MNP.
According to all these figures, it is observed that (1) the cell viability of MNP or HAP with
low (100 ?g/mL) concentration is high, (2) for MNP, viability increased with concentrations
(Fig 4D?4F), so 1000 ?g/mL was the highest one, (3) for HAP, viability is highest in the
500 ?g/mL group (Fig 4G?4I).
This result contradicts with previous studies where researchers demonstrated the positive
effect of HAP on osteoblast proliferation and differentiation [
]. However, other
researchers provided evidence that cell viability is related to HAP concentration. The HAP induced a
negative effect on osteoblast functions which strongly suggests phagocytosis process. The
phagocytosis process produces an accumulation of calcium in mitochondria and eventually
leads to mitochondria lysis and cell death . Therefore, selecting the better concentration
range of HAP is crucial for improving osteoblast activity without compromising cell viability.
8 / 17
Fig 4. After day 7, the cell viability of co-culturing with different inorganic nanoparticles: (A) control, (B) MNP
100 ?g/mL, (C) HAP 100 ?g/mL, (D) MNP 500 ?g/mL, (E) MNP 750 ?g/mL, (F) MNP 1000 ?g/mL, (G) HAP 500 ?g/
mL, (H) HAP 750 ?g/mL, and (I) HAP 1000 ?g/mL.
Finally, concentrations of HAP and MNP were fixed at 500 ?g/mL and 1000 ?g/mL,
To examine the surface and interior morphologies of the hydrogels, SEM microscopy was
adopted. Fig 5A, 5B, 5C and 5D show the microstructure of lyophilized 3% hydrogels of mPA,
M10/mPA, H1/mPA, and H5/mPA respectively. As shown in Fig 5A, 5B and 5C, lyophilized
hydrogels exhibited a plate-like 3D structure. However, when a high concentration of HAP
was used, the plate-like structure became more porous. The porous structure allows not only
the transport of nutrients, oxygen, carbon dioxide, and metabolite but also provides space for
cell proliferation during 3D cell culture [
]. The pore size differed depending on the type of
encapsulated inorganic nanoparticles [
]. When particles encapsulated in di-block
hydrogels are confined between two surfaces, the effects of chain stretching play an important role.
Lee et al.  showed that a symmetric AB diblock copolymer confined between two surfaces
forms a lamellar structure. The micro domain of stripes are oriented either parallel or
perpendicular to the layers. Lin et al. [
] experimental studies showed precisely this behavior of
mediated interfacial interactions, and reoriented micro domains. Finally, nanoparticles were
excluded to the surfaces and caused the micro domains to orient normal to the surface. In our
study, we observed a similar behavior when different concentrations of nanoparticle were
encapsulated into the hydrogel. As shown in Fig 5C, low concentration of HAP did not change
the hydrogel structure. However, a porous transformation was noted in Fig 5D and 5E. This
suggests that high concentration of HAP prevents adequate dispersion and thus HAP were
excluded to the hydrogel surface. The aggregation of HAP likely destroys the sheet-like
structure, causing the gel to adopt a more porous structure.
Although the incorporation of HAP increased the porosity of the scaffold, high
concentration HAP decreased the cell viability. Therefore, proper concentrations of MNP and HAP
were chosen, as mentioned before.
9 / 17
Fig 5. The SEM images of (A) mPA (blank), (B) M10/mPA (mPA+ 1000 ?g/mL MNP), (C) H1/mPA (mPA+ 100 ?g/mL
HAP), (D) H5/mPA (mPA + 500 ?g/mL HAP) hydrogels, and (E) the magnification of H5/mPA.
Sol-gel transition and FTIR measurement for secondary structure
Rheological properties of a 3% (w/v) aqueous solution of various composite hydrogels are as
shown in Fig 6A, 6B and 6C. The gelation temperature corresponding to the crossover point of
G? and G? were at 28.0?C, 27.0?C, and 23.5?C respectively for mPA, M10/mPA, and H5/mPA.
Su et al. [
] studied the gelation and bioactivity behavior of an injectable silk fibroin hydrogel
with laponite nanoplatelets (LAP), concluding that LAP served as both a medium to accelerate
the hydrophobic interactions among silk fibroin and a disruptor to limit the growth of ?-sheet
domain during the gelation. Corresponding secondary structures found in nanocomposite
hydrogels at 37?C are shown in Fig 6D. Result shows that HAP incorporation was disruptive
and decreased the proportion of random coils and ?-helix. The lowering of storage modulus,
as shown in Fig 6A, 6B and 6C, could be attributed to the same mechanism.
10 / 17
Fig 6. Dynamic rheology measurements: Storage modulus (G0) and loss modulus (G00) of (A) mPA, (B) M10/mPA,
(C) H5/mPA as a function of temperature. (D) The FTIR spectra of mPA, H5/mPA, and M10/mPA hydrogels.
LIVE/DEAD staining of gel-encapsulated cells
LIVE/DEAD staining revealed that the cells were metabolically active and homogenously
distributed within the hydrogel matrix at different time point. (Fig 7) With extended culture, the
number of viable cells increased in all hydrogels. However, in 3D culture groups (Fig 7B, 7C
and 7D), osteoblasts migrated into clusters on day 21 and the hydrogel became opaque
compared to the control (Fig 7A), likely owing to the accumulation of ECM material and/or
]. The ECM is a combination of numerous components, which jointly provide a wide
range of functionality. Except for providing structural support, the ECM is also a channel for
cell-cell communication [
], and a driving force behind organogenesis [
Previous studies also demonstrated that ECM mineralization could be induced by the
addition of inorganic nanoparticles that provide attachment sites to enhance integration with
surrounding bone tissue [
]. Furthermore, we also observed the characteristic of MC3T3-E1
cells differentiation such as microfilaments. The hydrogel encapsulated with HAP (Fig 7C in
day 14) and MNP (Fig 7D in day 14) compared with mPA (Fig 7B in day 14), we observed
more microfilaments in groups with nanoparticles than mPA group. This kind of change in
cell morphology was also observed in previous studies [
Fig 7. The live/dead staining images of (A) control (2D culture), (B) mPA, (C) H5/mPA, and (D) M10/mPA after day
7, 14, and 21 cultured. (B, C, D were 3D culture).
11 / 17
Fig 8. (A) OPN, (B) OCN, and (C) ALP gene expressions as a function of time. GAPDH was used as the housekeeping
gene. ?+? denotes the presence of a static magnetic field.
Biochemical analysis and real time-PCR of gel-encapsulated cells under
Static magnetic field. The three main characteristics of cellular growth during
differentiation from pre-osteoblasts to osteoblasts are cell proliferation, ECM maturation and
]. The expression of osteoblast proliferation and differentiation markers, OPN, OCN
and ALP, were analyzed by real time PCR as shown in Fig 8. ALP activity is an early marker
(before 14 days) for osteogenic differentiation and regulates phosphate metabolism [
our experimental design, the LA-ICPMS test samples were used the 48 well plate space to
analysis the dispersion of nanoparticles in the hydrogel. So, we also used the 48 well plate to form
the similar hydrogel to conduct our gene expression experiments. As shown in Fig 8, ALP
activity was induced after 14 days of culture in all test groups. A significant 1-fold increase in
ALP activity was observed when a static magnetic field was applied on M10/mPA. Injectable
polypeptide hydrogels have been shown to provide a suitable environment for cell attachment
and growth by mimicking the structure of ECM [
]. In this study, MNP was
incorporated into the polypeptide hydrogel, to render responsively to an applied magnetic field. MNP
as an intrinsic component of the polypeptide hydrogel allows the introduction of magnetic
force inside the hydrogel when an external magnetic is introduced. This magnetic force
continuously stimulates proliferation of osteoblasts and secretion of new ECM [
studies reported that in common cell culture systems, weak magnetic force with an intensity of
0.1?10 T accelerated osteoblast differentiation [
29, 66, 67
After the expression of ALP, osteoblasts begin to develop and mature. At the stage of bone
matrix maturation and mineralization, osteoblasts express high levels of OPN which
modulates the mineralization of the bone matrix. OPN is a highly acidic phosphoprotein that is
related to cell adhesion [
]. Meanwhile, because OPN is a secreted protein, high levels of
ECM easily sequester OPN within the polypeptide hydrogel. Results show that without an
applied magnetic field, cells cultured in H5/mPA showed higher expression level of OPN
beginning on day 14 and continued to day 21 compared to the other groups. In addition, OPN
upregulation was observed with prolonged culture. The expression of OPN in all groups was
increased approximately two- to three-folds.
Fig 9. Real time RT-PCR analysis of (A) OPN, (B) OCN, and (C) ALP gene expressions on day 21 with the application
of a moving magnetic field. GAPDH was used as the housekeeping gene. The representation ?+? means applied the
moving magnetic field.
12 / 17
However, when a static magnetic field was applied, cells cultured in M10/mPA exhibited
higher expression level of OPN compared to H5/mPA and the other groups. OCN is a small
protein produced by osteoblasts during the development period of extracellular matrix
mineralization and it is also a late biomarker. As shown, its expression was highest after 21 days of
incubation. A two-fold increase was noted in M10/mPA and H5/mPA from day 14 to day 21.
Although the precise function of OPN and OCN are not fully elucidated, previous studies
demonstrated that they play an important role in calcium decomposition and mineralization
The gene expression of ALP, OPN, and OCN in the H5/mPA group was higher than that of
other groups and this can be attributed to the positive effect of calcium ions released into the
culture medium by HAP. On the other hand, the application of external magnetic fields shown
to positively affect bone regeneration in all group, though not as large as those HAP or MNP
induced. The major effect of SMF on osteoblast differentiation is inducing membrane
reorientation and distortion, which alter the diamagnetic isotropic properties [
]. The SMF changes
cell-cell contact properties in confluent or post-confluent cultures. This change correlates to
the reorientation of phospholipids which results in the deformation of the lipid bilayer or
proteins embedded on the membrane [
Moving magnetic field. A moving magnetic field was used to stimulate the culture
osteoblasts and a pulsed exposure scheme was designed to prevent overheating of the mechanical
shaker. By referencing previous studies, a daily exposure time of 60 minutes for 21 days was
]. Compare to the results of static magnetic field, similar findings were observed
with the use of a moving magnetic field, as shown in Fig 9. When a moving magnetic field was
applied, OPN and OCN expressions were increased. Encapsulated MNP likely acted as
substrates that attract growth factors in a magnetic guiding process . Furthermore,
encapsulated MNP also is capable of acting as a cross-linking agent, providing chemical-physical
In this work, a simple method for encapsulating different inorganic nanoparticles in a
polypeptide hydrogel was reported. Cell culture results confirmed the compatibility of these
hydrogels with pre-osteoblasts. PCR results demonstrated that HAP acted as a proliferation cue in
H5/mPA hydrogel and ALP expression was upregulated in the same system. Application of a
magnetic field to cells encapsulated in MNP-incorporated polypeptide hydrogel showed
positive enhancement to osteoblast differentiation. The idea of nano-particle incorporation to
cellencasulating hydrogel was proved to be beneficial for bone regeneration in principle, and the
magnetic field?s positive effects on osteoblast differentiation were demonstrated.
We would like to thank the instrumentation center in National Taiwan University for TEM
Conceptualization: Wei-Shun Huang.
Data curation: Wei-Shun Huang.
Funding acquisition: Wei-Shun Huang.
Investigation: Wei-Shun Huang.
13 / 17
Methodology: Wei-Shun Huang.
Project administration: Wei-Shun Huang.
Resources: Wei-Shun Huang.
Software: Wei-Shun Huang.
Supervision: Wei-Shun Huang, I-Ming Chu.
Validation: Wei-Shun Huang.
Visualization: Wei-Shun Huang.
Writing ? original draft: Wei-Shun Huang.
Writing ? review & editing: Wei-Shun Huang, I-Ming Chu.
14 / 17
15 / 17
16 / 17
1. Liu G , Zhao L , Zhang W , Cui L , Liu W , Cao Y. Repair of goat tibial defects with bone marrow stromal cells and ?-tricalcium phosphate . Journal of Materials Science: Materials in Medicine . 2008 ; 19 ( 6 ): 2367 - 76 . https://doi.org/10.1007/s10856-007 -3348-3 PMID: 18158615
2. Gao T , Lindholm T , Kommonen B , Ragni P , Paronzini A , Lindholm T , et al. Enhanced healing of segmental tibial defects in sheep by a composite bone substitute composed of tricalcium phosphate cylinder, bone morphogenetic protein, and type IV collagen . Journal of Biomedical Materials Research Part A . 1996 ; 32 ( 4 ): 505 - 12 .
3. Place ES , George JH , Williams CK , Stevens MM . Synthetic polymer scaffolds for tissue engineering . Chemical Society Reviews . 2009 ; 38 ( 4 ): 1139 - 51 . https://doi.org/10.1039/b811392k PMID: 19421585
4. Lee S-H , Shin H. Matrices and scaffolds for delivery of bioactive molecules in bone and cartilage tissue engineering . Advanced drug delivery reviews . 2007 ; 59 ( 4 ): 339 - 59 .
5. Lutolf M , Hubbell J . Synthetic biomaterials as instructive extracellular microenvironments for morphogenesis in tissue engineering . Nature biotechnology . 2005 ; 23 ( 1 ): 47 - 55 . https://doi.org/10.1038/ nbt1055 PMID: 15637621
6. Klouda L , Mikos AG . Thermoresponsive hydrogels in biomedical applications . European Journal of Pharmaceutics and Biopharmaceutics . 2008 ; 68 ( 1 ): 34 - 45 . https://doi.org/10.1016/j.ejpb. 2007 . 02 .025 PMID: 17881200
7. Chung HJ , Park TG . Self-assembled and nanostructured hydrogels for drug delivery and tissue engineering . Nano Today . 2009 ; 4 ( 5 ): 429 - 37 .
8. Klok H-A , Langenwalter JF , Lecommandoux S . Self-assembly of peptide-based diblock oligomers . Macromolecules . 2000 ; 33 ( 21 ): 7819 - 26 .
9. Oh HJ , Joo MK , Sohn YS , Jeong B . Secondary structure effect of polypeptide on reverse thermal gelation and degradation of L/DL-Poly (alanine)-poloxamer-L/DL-poly (alanine) copolymers . Macromolecules. 2008 ; 41 ( 21 ): 8204 - 9 .
10. Dankers PY , Meijer E. Supramolecular biomaterials. A modular approach towards tissue engineering . Bulletin of the Chemical Society of Japan . 2007 ; 80 ( 11 ): 2047 - 73 .
11. Schexnailder P , Schmidt G . Nanocomposite polymer hydrogels . Colloid and Polymer Science . 2009 ; 287 ( 1 ): 1 - 11 .
12. Haraguchi K , editor Nanocomposite gels: new advanced functional soft materials . Macromolecular Symposia; 2007 : Wiley Online Library. https://doi.org/10.1002/masy.200750318 PMID: 20930942
13. Haraguchi K. Nanocomposite hydrogels . Current Opinion in Solid State and Materials Science . 2007 ; 11 ( 3 ): 47 - 54 .
14. Oliveira JM , Rodrigues MT , Silva SS , Malafaya PB , Gomes ME , Viegas CA , et al. Novel hydroxyapatite/chitosan bilayered scaffold for osteochondral tissue-engineering applications: Scaffold design and its performance when seeded with goat bone marrow stromal cells . Biomaterials . 2006 ; 27 ( 36 ): 6123 - 37 . https://doi.org/10.1016/j.biomaterials. 2006 . 07 .034 PMID: 16945410
15. Deville S , Saiz E , Tomsia AP . Freeze casting of hydroxyapatite scaffolds for bone tissue engineering . Biomaterials . 2006 ; 27 ( 32 ): 5480 - 9 . https://doi.org/10.1016/j.biomaterials. 2006 . 06 .028 PMID: 16857254
16. Panseri S , Russo A , Giavaresi G , Sartori M , Veronesi F , Fini M , et al. Innovative magnetic scaffolds for orthopedic tissue engineering . Journal of Biomedical Materials Research Part A . 2012 ; 100 ( 9 ): 2278 - 86 . https://doi.org/10.1002/jbm.a.34167 PMID: 22499413
17. Gloria A , Russo T , D'Amora U , Zeppetelli S , D'Alessandro T , Sandri M , et al. Magnetic poly (?-caprolactone)/iron-doped hydroxyapatite nanocomposite substrates for advanced bone tissue engineering . Journal of The Royal Society Interface . 2013 ; 10 ( 80 ): 20120833 .
18. Hou R , Zhang G , Du G , Zhan D , Cong Y , Cheng Y , et al. Magnetic nanohydroxyapatite/PVA composite hydrogels for promoted osteoblast adhesion and proliferation . Colloids and Surfaces B: Biointerfaces . 2013 ; 103 : 318 - 25 . https://doi.org/10.1016/j.colsurfb. 2012 . 10 .067 PMID: 23261554
19. Li Y , Huang G , Zhang X , Li B , Chen Y , Lu T , et al. Magnetic hydrogels and their potential biomedical applications . Advanced Functional Materials . 2013 ; 23 ( 6 ): 660 - 72 .
20. Gaharwar AK , Dammu SA , Canter JM , Wu C-J , Schmidt G . Highly extensible, tough, and elastomeric nanocomposite hydrogels from poly (ethylene glycol) and hydroxyapatite nanoparticles . Biomacromolecules . 2011 ; 12 ( 5 ): 1641 - 50 . https://doi.org/10.1021/bm200027z PMID: 21413708
Wongwitwichot P , Kaewsrichan J , Chua K , Ruszymah B . Comparison of TCP and TCP/HA hybrid scaffolds for osteoconductive activity . The open biomedical engineering journal . 2010 ; 4 : 279 . https://doi. org/10.2174/1874120701004010279 PMID: 21625376
22. Armentano I , Dottori M , Fortunati E , Mattioli S , Kenny J . Biodegradable polymer matrix nanocomposites for tissue engineering: a review . Polymer degradation and stability . 2010 ; 95 ( 11 ): 2126 - 46 .
23. Meng J , Xiao B , Zhang Y , Liu J , Xue H , Lei J , et al. Super-paramagnetic responsive nanofibrous scaffolds under static magnetic field enhance osteogenesis for bone repair in vivo . Scientific reports . 2013 ; 3 .
24. Panseri S , Russo A , Sartori M , Giavaresi G , Sandri M , Fini M , et al. Modifying bone scaffold architecture in vivo with permanent magnets to facilitate fixation of magnetic scaffolds . Bone . 2013 ; 56 ( 2 ): 432 - 9 . https://doi.org/10.1016/j.bone. 2013 . 07 .015 PMID: 23876980
25. Zeng XB , Hu H , Xie LQ , Lan F , Jiang W , Wu Y , et al. Magnetic responsive hydroxyapatite composite scaffolds construction for bone defect reparation . International journal of nanomedicine . 2012 ; 7 : 3365 . https://doi.org/10.2147/IJN.S32264 PMID: 22848165
26. Bock N , Riminucci A , Dionigi C , Russo A , Tampieri A , Landi E , et al. A novel route in bone tissue engineering: magnetic biomimetic scaffolds . Acta Biomaterialia . 2010 ; 6 ( 3 ): 786 - 96 . https://doi.org/10.1016/ j.actbio. 2009 . 09 .017 PMID: 19788946
27. Fu Y-C , Lin C-C, Chang J-K, Chen C-H, Tai I-C , Wang G-J , et al. A novel single pulsed electromagnetic field stimulates osteogenesis of bone marrow mesenchymal stem cells and bone repair . PloS one . 2014 ; 9 ( 3 ):e91581. https://doi.org/10.1371/journal.pone. 0091581 PMID: 24632682
28. Xy Zhang , Xue Y , Zhang Y. Effects of 0.4 T rotating magnetic field exposure on density, strength, calcium and metabolism of rat thigh bones . Bioelectromagnetics . 2006 ; 27 ( 1 ): 1 - 9 . https://doi.org/10.1002/ bem.20165 PMID: 16304694
29. Kotani H , Kawaguchi H , Shimoaka T , Iwasaka M , Ueno S , Ozawa H , et al. Strong static magnetic field stimulates bone formation to a definite orientation in vitro and in vivo . Journal of Bone and Mineral Research . 2002 ; 17 ( 10 ): 1814 - 21 . https://doi.org/10.1359/jbmr. 2002 . 17 .10. 1814 PMID: 12369785
30. Choi YY , Joo MK , Sohn YS , Jeong B . Significance of secondary structure in nanostructure formation and thermosensitivity of polypeptide block copolymers . Soft Matter . 2008 ; 4 ( 12 ): 2383 - 7 .
31. Peng S , Wu C-W , Lin J-Y , Yang C -Y, Cheng M-H , Chu I-M . Promoting chondrocyte cell clustering through tuning of a poly (ethylene glycol)-poly (peptide) thermosensitive hydrogel with distinctive microarchitecture . Materials Science and Engineering: C. 2017 ; 76 : 181 - 9 .
32. Cheng F-Y, Su C-H , Yang Y-S , Yeh C-S , Tsai C-Y , Wu C-L , et al. Characterization of aqueous dispersions of Fe 3 O 4 nanoparticles and their biomedical applications . Biomaterials . 2005 ; 26 ( 7 ): 729 - 38 . https://doi.org/10.1016/j.biomaterials. 2004 . 03 .016 PMID: 15350777
33. Zhao R , Yang X , Chen C , Chen K , Wang S , Xie C , et al. The anti-tumor effect of p53 gene-loaded hydroxyapatite nanoparticles in vitro and in vivo . Journal of Nanoparticle Research . 2014 ; 16 ( 4 ): 2353 .
34. Luo F , Hou T , Zhang Z , Xie Z , Wu X , Xu J. Effects of pulsed electromagnetic field frequencies on the osteogenic differentiation of human mesenchymal stem cells . Orthopedics . 2012 ; 35 ( 4 ): e526 - e31 . https://doi.org/10.3928/ 01477447 -20120327-11 PMID: 22495854
35. Chou YF , Dunn JC , Wu BM . In vitro response of MC3T3-E1 preosteoblasts within three-dimensional apatite-coated PLGA scaffolds . Journal of Biomedical Materials Research Part B: Applied Biomaterials . 2005 ; 75 ( 1 ): 81 - 90 . https://doi.org/10.1002/jbm.b. 30261 PMID: 16001421
36. Hamley I. Nanotechnology with soft materials . Angewandte Chemie International Edition . 2003 ; 42 ( 15 ): 1692 - 712 . https://doi.org/10.1002/anie.200200546 PMID: 12707884
37. Sun C , Veiseh O , Gunn J , Fang C , Hansen S , Lee D , et al. In vivo MRI detection of gliomas by chlorotoxin-conjugated superparamagnetic nanoprobes . small . 2008 ; 4 ( 3 ): 372 - 9 . https://doi.org/10.1002/ smll.200700784 PMID: 18232053
38. Lee H , Yu MK , Park S , Moon S , Min JJ , Jeong YY , et al. Thermally cross-linked superparamagnetic iron oxide nanoparticles: synthesis and application as a dual imaging probe for cancer in vivo . Journal of the American Chemical Society . 2007 ; 129 ( 42 ): 12739 - 45 . https://doi.org/10.1021/ja072210i PMID: 17892287
39. Chirinos JR , Oropeza DD , Gonzalez JJ , Hou H , Morey M , Zorba V , et al. Simultaneous 3-dimensional elemental imaging with LIBS and LA-ICP-MS . Journal of Analytical Atomic Spectrometry . 2014 ; 29 ( 7 ): 1292 - 8 .
40. Pozebon D , Scheffler GL , Dressler VL , Nunes MA . Review of the applications of laser ablation inductively coupled plasma mass spectrometry (LA-ICP-MS) to the analysis of biological samples . Journal of Analytical Atomic Spectrometry . 2014 ; 29 ( 12 ): 2204 - 28 .
41. Karadzic I , Vucic V , Jokanovic V , Debeljak-Martacic J , Markovic D , Petrovic S , et al. Effects of novel hydroxyapatite-based 3D biomaterials on proliferation and osteoblastic differentiation of mesenchymal stem cells . Journal of Biomedical Materials Research Part A . 2015 ; 103 ( 1 ): 350 - 7 . https://doi.org/10. 1002/jbm.a.35180 PMID: 24665062
42. Uskokovi? V , Batarni SS , Schweicher J , King A , Desai TA . Effect of calcium phosphate particle shape and size on their antibacterial and osteogenic activity in the delivery of antibiotics in vitro . ACS applied materials & interfaces . 2013 ; 5 ( 7 ): 2422 - 31 .
43. Li L , Pan H , Tao J , Xu X , Mao C , Gu X , et al. Repair of enamel by using hydroxyapatite nanoparticles as the building blocks . Journal of Materials Chemistry . 2008 ; 18 ( 34 ): 4079 - 84 .
44. Pioletti DP , Takei H , Lin T , Van Landuyt P , Ma QJ , Kwon SY , et al. The effects of calcium phosphate cement particles on osteoblast functions . Biomaterials . 2000 ; 21 ( 11 ): 1103 - 14 . PMID: 10817262
45. Remya N , Syama S , Gayathri V , Varma H , Mohanan P. An in vitro study on the interaction of hydroxyapatite nanoparticles and bone marrow mesenchymal stem cells for assessing the toxicological behaviour . Colloids and Surfaces B: Biointerfaces . 2014 ; 117 : 389 - 97 . https://doi.org/10.1016/j.colsurfb. 2014 . 02 . 004 PMID: 24675277
46. Kim U , Shu C-W , Dane KY , Daugherty PS , Wang JY , Soh H . Selection of mammalian cells based on their cell-cycle phase using dielectrophoresis . Proceedings of the National Academy of Sciences . 2007 ; 104 ( 52 ): 20708 - 12 .
47. Mohan YM , Lee K , Premkumar T , Geckeler KE . Hydrogel networks as nanoreactors: A novel approach to silver nanoparticles for antibacterial applications . Polymer . 2007 ; 48 ( 1 ): 158 - 64 .
48. Lee JY , Shou Z , Balazs AC . Modeling the self-assembly of copolymer-nanoparticle mixtures confined between solid surfaces . Physical review letters . 2003 ; 91 ( 13 ): 136103 . https://doi.org/10.1103/ PhysRevLett.91.136103 PMID: 14525321
49. Lin Y , Bo? ker A , He J , Sill K , Xiang H , Abetz C , et al. Self-directed self-assembly of nanoparticle/copolymer mixtures . Nature . 2005 ; 434 ( 7029 ): 55 . https://doi.org/10.1038/nature03310 PMID: 15744296
50. Su D , Jiang L , Chen X , Dong J , Shao Z. Enhancing the gelation and bioactivity of injectable silk fibroin hydrogel with laponite nanoplatelets . ACS applied materials & interfaces . 2016 ; 8 ( 15 ): 9619 - 28 .
51. Wu AT , Aoki T , Sakoda M , Ohta S , Ichimura S , Ito T , et al. Enhancing osteogenic differentiation of MC3T3-E1 cells by immobilizing inorganic polyphosphate onto hyaluronic acid hydrogel . Biomacromolecules . 2014 ; 16 ( 1 ): 166 - 73 . https://doi.org/10.1021/bm501356c PMID: 25423088
52. Fan D , Creemers EE , Kassiri Z. Matrix as an interstitial transport system . Circulation research . 2014 ; 114 ( 5 ): 889 - 902 . https://doi.org/10.1161/CIRCRESAHA.114.302335 PMID: 24577968
53. Sakai T , Larsen M , Yamada KM . Fibronectin requirement in branching morphogenesis . Nature . 2003 ; 423 ( 6942 ): 876 . https://doi.org/10.1038/nature01712 PMID: 12815434
54. Rea S , Best S , Bonfield W. Bioactivity of ceramic-polymer composites with varied composition and surface topography . Journal of Materials Science: Materials in Medicine . 2004 ; 15 ( 9 ): 997 - 1005 . https:// doi.org/10.1023/B:JMSM. 0000042685 .63383.86 PMID: 15448407
55. Dorozhkin SV , Epple M. Biological and medical significance of calcium phosphates . Angewandte Chemie International Edition . 2002 ; 41 ( 17 ): 3130 - 46 . https://doi.org/10.1002/ 1521 - 3773 ( 20020902 ) 41: 17 < 3130 : : AID -ANIE3130>3.0.CO;2-1 PMID: 12207375
56. Swetha M , Sahithi K , Moorthi A , Srinivasan N , Ramasamy K , Selvamurugan N. Biocomposites containing natural polymers and hydroxyapatite for bone tissue engineering . International journal of biological macromolecules . 2010 ; 47 ( 1 ): 1 - 4 . https://doi.org/10.1016/j.ijbiomac. 2010 . 03 .015 PMID: 20361991
57. Park MH , Yu Y , Moon HJ , Ko DY , Kim HS , Lee H , et al. 3D Culture of Tonsil-Derived Mesenchymal Stem Cells in Poly (ethylene glycol)-Poly (l-alanine-co-l-phenyl alanine) Thermogel. Advanced healthcare materials . 2014 ; 3 ( 11 ): 1782 - 91 . https://doi.org/10.1002/adhm.201400140 PMID: 24958187
58. Li D , Sun H , Jiang L , Zhang K , Liu W , Zhu Y , et al. Enhanced biocompatibility of PLGA nanofibers with gelatin/nano-hydroxyapatite bone biomimetics incorporation . ACS applied materials & interfaces . 2014 ; 6 ( 12 ): 9402 - 10 .
59. Tsutsumi K , Saito N , Kawazoe Y , Ooi H-K , Shiba T. Morphogenetic study on the maturation of osteoblastic cell as induced by inorganic polyphosphate . PLoS One . 2014 ; 9 ( 2 ):e86834. https://doi.org/10. 1371/journal.pone. 0086834 PMID: 24498284
60. Stein GS , Lian JB , Stein JL , Van Wijnen AJ , Montecino M. Transcriptional control of osteoblast growth and differentiation . Physiological reviews . 1996 ; 76 ( 2 ): 593 - 629 . https://doi.org/10.1152/physrev. 1996 . 76 .2.593 PMID: 8618964
61. Stein GS , Lian JB , Owen TA . Relationship of cell growth to the regulation of tissue-specific gene expression during osteoblast differentiation . The FASEB journal . 1990 ; 4 ( 13 ): 3111 - 23 . PMID: 2210157
62. Ren K , Cui H , Xu Q , He C , Li G , Chen X . Injectable Polypeptide Hydrogels with Tunable Microenvironment for 3D Spreading and Chondrogenic Differentiation of Bone-Marrow-Derived Mesenchymal Stem Cells . Biomacromolecules . 2016 ; 17 ( 12 ): 3862 - 71 . https://doi.org/10.1021/acs.biomac. 6b00884 PMID: 27775890
63. Zhang Y-X , Chen Y-F , Shen X-Y , Hu J-J , Jan J-S. Reduction-and pH-Sensitive lipoic acid-modified Poly (l-lysine) and polypeptide/silica hybrid hydrogels/nanogels . Polymer. 2016 ; 86 : 32 - 41 .
64. Kim S-J , Park MH , Moon HJ , Park JH , Ko DY , Jeong B . Polypeptide thermogels as a three dimensional culture scaffold for hepatogenic differentiation of human tonsil-derived mesenchymal stem cells . ACS applied materials & interfaces . 2014 ; 6 ( 19 ): 17034 - 43 .
65. Galler KM , Aulisa L , Regan KR , D'Souza RN , Hartgerink JD . Self-assembling multidomain peptide hydrogels: designed susceptibility to enzymatic cleavage allows enhanced cell migration and spreading . Journal of the American Chemical Society . 2010 ; 132 ( 9 ): 3217 - 23 . https://doi.org/10.1021/ja910481t PMID: 20158218
66. Kim EC , Leesungbok R , Lee SW , Lee HW , Park SH , Mah SJ , et al. Effects of moderate intensity static magnetic fields on human bone marrow-derived mesenchymal stem cells . Bioelectromagnetics . 2015 ; 36 ( 4 ): 267 - 76 . https://doi.org/10.1002/bem.21903 PMID: 25808160
67. Huang H-M , Lee S-Y , Yao W-C , Lin C-T , Yeh C-Y. Static magnetic fields up-regulate osteoblast maturity by affecting local differentiation factors . Clinical orthopaedics and related research . 2006 ; 447 : 201 - 8 . https://doi.org/10.1097/01.blo. 0000203464 .35561. be PMID : 16456312
68. Liu Y-K , Uemura T , Nemoto A , Yabe T , Fujii N , Ushida T , et al. Osteopontin involvement in integrinmediated cell signaling and regulation of expression of alkaline phosphatase during early differentiation of UMR cells . FEBS letters . 1997 ; 420 ( 1 ): 112 - 6 . PMID: 9450560
69. Seibel MJ . Biochemical markers of bone turnover part I: biochemistry and variability . The Clinical biochemist Reviews/Australian Association of Clinical Biochemists . 2005 ; 26 ( 4 ): 97 .
70. McDonald F . Effect of static magnetic fields on osteoblasts and fibroblasts in vitro . Bioelectromagnetics . 1993 ; 14 ( 3 ): 187 - 96 . PMID: 8323569
71. Yamamoto Y , Ohsaki Y , Goto T , Nakasima A , Iijima T. Effects of static magnetic fields on bone formation in rat osteoblast cultures . Journal of dental research . 2003 ; 82 ( 12 ): 962 - 6 . https://doi.org/10.1177/ 154405910308201205 PMID: 14630895
72. Ceccarelli G , Bloise N , Mantelli M , Gastaldi G , Fassina L , Cusella De Angelis MG , et al. A comparative analysis of the in vitro effects of pulsed electromagnetic field treatment on osteogenic differentiation of two different mesenchymal cell lineages . BioResearch open access . 2013 ; 2 ( 4 ): 283 - 94 . https://doi.org/ 10.1089/biores. 2013 .0016 PMID: 23914335
73. Zhou J , Ming L-G , Ge B-F , Wang J-Q , Zhu R-Q , Wei Z , et al. Effects of 50Hz sinusoidal electromagnetic fields of different intensities on proliferation, differentiation and mineralization potentials of rat osteoblasts . Bone . 2011 ; 49 ( 4 ): 753 - 61 . https://doi.org/10.1016/j.bone. 2011 . 06 .026 PMID: 21726678
74. Tampieri A , Landi E , Valentini F , Sandri M , D'alessandro T , Dediu V , et al. A conceptually new type of bio-hybrid scaffold for bone regeneration . Nanotechnology . 2010 ; 22 ( 1 ): 015104 . https://doi.org/10. 1088/ 0957 -4484/22/1/015104 PMID: 21135464